DAMAGE MECHANICS MODELING OF CONCURRENT THERMAL AND VIBRATION LOADING ON ELECTRONICS PACKAGING


 Coleen Dixon
 1 years ago
 Views:
Transcription
1 Multidiscipline Modeling in Mat. and Str., Vol. 2, No.3, pp (2006) BRILL Also available onlinewww.vsppub.com DAMAGE MECHANICS MODELING OF CONCURRENT THERMAL AND VIBRATION LOADING ON ELECTRONICS PACKAGING Juan Gomez 1, Minghui Lin 1 and Cemal Basaran 2 1 Research Assistant, UB Electronic Packaging Laboratory. 2 Professor, and Director, UB Electronic Packaging Laboratory University at Buffalo, State University of New York Received 3 February 2005; accepted 26 October 2005 Abstract The problem of concurrent thermal and vibration loading has not been thoroughly studied even though it is common in electronic packaging applications. Here we attempt to address such a problem using a damage mechanics based constitutive model. Damage mechanics constitutive model for eutectic Pb/Sn solder alloys is used to simulate the damage effects of concurrent cyclic thermal loads and vibrations on Ball Grid Array (BGA) packages. The model is implemented into the commercial finite element code ABAQUS through its user defined material subroutine capability. For the integration algorithm we have used a return mapping scheme, which dramatically improves the convergency rate as compared to previous implementations of the same model. Results are examined in terms of accumulation of plastic strain within the solder connections. It is shown that the simplistic Miner s rule can not accurately account for the combined effect of both loadings acting concurrently. Keywords: Finite element analysis, constitutive model, dynamic analysis, concurrent loading, microelectronics packaging, solder joints. 1. INTRODUCTION The most common mode of failure in microelectronic packaging solder joints is low cycle fatigue. Temperature changes and the coefficient of thermal expansion mismatch between the soldered parts is the main reason behind the fatigue. When an electronic package undergoes a temperature variation interconnects are stressed mainly in cyclic shear. The stresses impart elastic and inelastic strains, which are also cyclic in nature leading to thermo mechanical fatigue. The temperatures changes are due to switch on/off operations or sometimes owing to fluctuations in the ambient conditions. On the other hand, eutectic solder alloys are routinely used at high homologous temperatures. The melting point of the eutectic Sn/Pb solder alloy is 183 C, and it is at 0.65T m at room temperature, where T m is the melting point. Therefore, solder joints exhibit time, temperature, stress dependent deformation behavior and such coupling makes constitutive modeling a difficult task. Material models ranging from purely elastic to elastoviscoplastic using various stressstrain relations have been proposed for Sn/Pb
2 310 Juan Gomez, Minghui Lin and Cemal Basaran solder alloys, such as in Kitano et al.(1988),[1], Lau & Rice(1990),[2], Basaran et al.(1998),[3] and many others. Adams (1986), [4] proposed a simple viscoplastic model without hardening. Wilcox et al (1989), [5], proposed a rheological model to represent the inelastic behavior of the material, however it is applicable to a limited range of strain rates. The purely phenomenological models proposed by Knocht and Fox (1990), [6], Darveaux and Banerji (1992), [7] and Hong and Burrell (1995), [8] decoupled the creep and plasticity effects artificially. This decoupling does not have any physical basis and is just motivated by mathematical convenience. Classical forms of decoupled plasticity and creep theories have been shown to be quite inferior for modeling cyclic plasticity, creep and interaction effects, Mcdowell et al(1994),[9]. Recently, Zhao(2000),[10], followed by Basaran and Tang (2002), [11] and Tang (2002), [12] have extended a creep law originally proposed by Kashyap and Murty(1998), [13] for eutectic solder alloys into a thermodynamics based framework for low cycle fatigue predictions. The model has been validated against thermomechanical fatigue experiments, Gomez and Basaran, (2005a), [14], performed on thin layer solder joints and nanoindentation experiments at room temperature, Gomez and Basaran (2005b), [15]. Another source of failure in electronic equipment is vibrations, Steinberg (2000), [16]. It is common for electronic equipment to be subjected to vibrations over a wide range of frequencies and acceleration levels. For instance, according to the US Air Force, vibration and shock loads are responsible for the mechanical failure of 20 percent of airborne electronics. These vibrations may occur simultaneously with thermal loads at some time during the service life of the structure. However, this combined effect has not been thoroughly studied or understood by the electronic packaging community, Basaran et al (2001), [17]. This is in part because of the lack of robust constitutive models to predict the creepvibrationfatigue interaction effects on eutectic solder alloys. Also the vibration and thermal cycling effects occur at different time scales which make the computational treatment highly expensive. On the other hand, there is not enough experimental data for verification of the computational models. In this paper we have implemented a constitutive model into the commercial finite element code ABAQUS through its user defined material subroutine capabilities. We have used a return mapping scheme as proposed in Simo and Hughes (1997), [18]. Previous ABAQUS implementations of similar models like in Tang(2002), [12], Basaran and Tang (2002), [11], Basaran et al(2005),[17] have made use of the Owen and Hinton(1980),[19] viscoplasticity integration scheme which when ported into ABAQUS exhibits very low convergence rate making it impractical if not impossible for dynamic loading applications. The main goal of the present paper is to study the combined effect of dynamic loads applied concurrently with thermal cycling. Although we do not directly calculate the fatigue life in our simulations, conclusions about the fatigue life are inferred from the computed inelastic strains and damage parameter under combined conditions. Experimentally, this problem was addressed by Zhao et al (1999), [20] where concurrent vibration and thermal cycling was performed on a commercial electronic package using a dynamic shaker embedded into a controlled thermal chamber. The effect on fatigue life of the concurrent loading conditions was described in terms of the plastic strains measured by high sensitivity Moire interferometer technique. Based on the boundary conditions, and loading profile they used it was concluded that the fatigue life is improved when the loads are applied concurrently and that the commonly used Miner s rule to superimpose the effects of the two loads acting independently is inaccurate. According to Barker et al (1990), [21],
3 Damage Mechanics Modeling of Concurrent Thermal. 311 Miner s rule, Miner (1945), [22] assumes that every structural member has a useful fatigue life and that every stress cycle uses up a part of this life. Furthermore, if the strains from vibrational and thermal loading are available, Miner s rule assumes that the nth nv fatigue life can be characterized like R = + where R is the ratio of number of N th N v cycles experienced n i to the fatigue life N i at a specific i th strain level. The fatigue life at a given strain level is commonly computed using CoffinManson relations or modified CoffinManson relations which was developed for structural steel. Miner s rule is intended as a first order approximation since it can not account for factors like creep and the temperature dependent dynamic properties of the structure. For instance, as the thermal load progresses certain parts of the package may soften or harden, leading also to changes in the natural frequencies of the structure and therefore to its dynamic response. However, we inhere show that even if the superposition trend of the Miner s rule is correct, it may not yield accurate results quantitatively when predicting fatigue life because it does not account for nonlinearities that may occur during the loading process. Moreover, we show here that Miner s rule may lead to nonconservative results. In order to prove our point we have conducted two sets of finite element analysis. First, we model a commercial personal computer PCB with all the mounted components where we conduct several analyses to show that the trend behind Miners rule is correct. Then we model a microprocessor package where we conduct several analyses to show that the trend behind Miner s rule is correct qualitatively. In this work we assume that the equivalent plastic strain reveals the damage trend even if it may not be quantitatively very accurate, Basaran et al (2005), [17]. 2. MATERIAL CONSTITUTIVE MODEL In the implemented constitutive model the return mapping scheme is the one after Simo and Hughes (1998), [18] and Lubarda and Benson (2002), [23] viscoplastic integration and the Alfano et al (2001), [24] scheme for the nonlinear kinematic hardening model are used. Damage is introduced using the effective stress concept and the strain equivalence principle. Rate dependent effects are considered by means of the viscous overstress concept. Here we present the flow theory formulation following the classical approach in terms of a yield function separating the elastic from the viscoplastic domain, a flow rule specifying the evolution of the viscoplastic strain, a set of hardening laws specifying the evolution of the hardening parameters and the evolution of damage like an additional state variable. In order to describe the model it is convenient to first present the equations for a rate independent material without any damage Hooke s Law For a classical Von Mises rate independent plasticity model with isotropic behavior Hooke s law reads p θ & σ = C & ε & ε & ε (1) : ( )
4 312 Juan Gomez, Minghui Lin and Cemal Basaran p where & ε, & ε and θ ε& are the rates of total strain, plastic strain and thermal strain respectively, C is the elastic constitutive tensor and : represents contraction between two tensors Yield surface The elastoplastic domain is defined according to the following yield function 2 F = S X K( α ) S X R( α) (2) 3 where F( σ, α ) is a yield surface separating the elastic from the inelastic domain, X is the deviatoric component of the back stress describing the position of the center of the yield surface in stress space, S is the deviatoric component of the stress tensor, 2 A A A represents the norm of a given tensor A, R( α ) K( α ) describes 3 the radius of the yield surface in stress space Flow rule The evolution of the plastic strain is represented by the general flow rule, P & ε = γ nˆ (3) F with nˆ = being the normal to the yield surface. σ 2.4. Isotropic hardening Isotropic hardening is described by the evolution of the radius of the yield surface according to 2 c K( α ) = Y0 + R ( 1 e α ) (4a) 3 where α is a plastic consistency parameter or plastic strain trajectory evolving according to (4b), Y 0 is the initial yield stress, R is an isotropic hardening saturation value and c is an isotropic hardening rate. 2 & α = γ (4b) The NonLinearKinematic Hardening (NLK) Rule The NLK rule is taken from Chaboche (1989), [25] and was originally proposed by Armstrong and Frederic (1966),[26]. Nonlinearities are introduced as a recall term to the Prager (1956), [27] linear rule. p X & = c & ε c X & α (5) 1 2
5 Damage Mechanics Modeling of Concurrent Thermal. 313 The first term represents the linear kinematic hardening as defined by Prager. The second term is a recall term, often called a dynamic recovery term, which introduces the nonlinearity between the back stress X and the actual plastic strain. When c 2 = 0 Eqn. (5) reduces to the linear kinematic rule. The NLK equation describes the rapid changes due to the plastic flow during cyclic loadings and plays an important role even under stabilized conditions (after saturation of cyclic hardening). In other words, these equations take into account the transient hardening effects in each stressstrain loop. After unloading, dislocation remobilization is implicitly described due to the back stress effect and the larger plastic modulus at the beginning of the reverse plastic flow Chaboche (1989), [25]. Note than in equation (5) c 1 corresponds to the term 2 C in the 3 original formulation and described in Basaran et al (2005), [17]. In the equations above, γ is a nonnegative plasticity (consistency) parameter representing the irreversible character of plastic flow and obeying the following properties. 1. For a rate independent material model γ obeys the socalled loading/unloading and consistency condition γ 0 and F( σ, α) 0 (6) γf( & σ, α ) = 0 (7) 2. For a rate dependent material model conditions (6) and (7) are replaced by a constitutive equation of the form. φ( F) γ = (8) η where η represents a viscosity material parameter. In the case of a rate independent material F satisfies conditions (6) and (7) and additionally stress states such F( σ, α ) > 0 are ruled out. In the case of a rate dependent material on the other hand, the magnitude of the viscoplastic flow is proportional to the distance of the stress state to the surface defined by F( σ, α ) = 0. Using this fact we have after using Eqn.(8) that the following relation can be established F =Θ ( γη ) (9) 1 Θ γη = φ γη. where ( ) ( ) 2.6. Viscoplastic creep law In this particular model the creep law is the one proposed by Kashyap and Murty (1981), [12] and extended to multiaxial case by Basaran and Tang (2002), [11] and given by n p vp AD0 Eb F b Q / Rθ F & εij = e (10) kθ E d σ ij where, A is a dimensionless material parameter which is temperature and rate dependent,
6 314 Juan Gomez, Minghui Lin and Cemal Basaran D Q/ Rθ i = D0e is a diffusion coefficient with 0 D representing a frequency factor, Q is the creep activation energy, R is the universal gas constant, θ is the absolute temperature in Kelvin, E( θ ) is a temperature dependent Young s modulus, b is the characteristic length of crystal dislocation (magnitude of Burger s vector), k is Boltzman s constant, d is the average grain size, p is a grain size exponent, n is a stress exponent for plastic deformation rate, where 1/n indicates strain sensitivity. p n kθ d Q/ Rθ From Eqn.(10) we can identify φ ( F) = F and η = e n 1. AD E b b 2.7. Damage coupled elastoviscoplastic model Making use of the strain equivalence principle we can write in the usual form, Lemaitre (1996), [28] vp θ & σ = 1 DC:( & ε & ε & ε ) (11) ( ) F = D 2 D S X ( 1 D) K( α ) S X 3 ( 1 D) R( α) (12) where D is a damage metric and D X = 1 D vp c ε c X α (13) 2.8. Formulation of damage function ( )( 1 2 ) Damage is considered following the approach by Basaran and Yan (1998), [29], Tang (2002), [12], Basaran and Nie (2004), [30], where the relation between the disorder and entropy established by Boltzmann using statistical mechanics and the second law of thermodynamics is exploited. Their thermodynamic framework assumes that damage and the disorder are analogous concepts and the thermodynamic disorder can be used to model the damage evolution. The damage formulation used here has the advantage over other damage formulations that is not derived from a damage potential and therefore there are not additional material properties. Thus, damage can be completely characterized using standard material properties. The Damage evolution function is given by D = 1 e (( e φ) /( N0kθ / ms )) D cr (14) where D cr is a damage threshold e φ is the difference between the changes in the internal energy and the Helmholtz free energy with respect to a reference state. This difference is obtained as follows: the internal energy equation, which is an expression of the first law of thermodynamics, reads de in ρ = σ ˆ ijdij + ργ qi, i (15) dt 0
7 Damage Mechanics Modeling of Concurrent Thermal. 315 in where D ij is the rate of deformation tensor. For the particular case of small strains and in dε in ij small displacements Dij =. ˆ γ is the internal heat production rate and q i is the dt rate of heat flux through the surface. The Helmholtz free energy is written in terms of the stress tensor thus dψ in ρ = σijdij (16) dt After combining Eqs. (15) and (16), the difference between the changes in the internal energy and the Helmholtz free energy with respect to a reference state is obtained as follows; t2 t2 t2 S in ij ij i, i t1 t1 t1 1 e φ = σ D dt + γdt q dt ρ (17) This damage evolution model and integration algorithm has been verified against nanoindentation and fatigue experiments performed at the UB electronic packaging lab under different temperatures and imposed displacement rate conditions, Basaran and Yan (1998), [29], Basaran and Tang (2002), [11], Gomez and Basaran (2003), [31]. 3. FINITE ELEMENT SIMULATION OF CONCURRENT LOADING ON A PRINTED CIRCUIT BOARD In order to study the response under concurrent thermal and vibration loads using the constitutive model described above we have modeled an actual electronic package using the commercial finite element code ABAQUS where the constitutive model has been implemented by a user subroutine UMAT.. The studied assembly consists of a personal computer Printed Circuit Board (PCB) with the most relevant components mounted. The PCB is approximately 305mm long x 270mm wide with a thickness of 1.6mm and made of epoxy fiberglass known as FR4. Properties for the materials other than solder joints are obtained from Pecht et al (1999), [32] and reported in Table 1. Pitarresi (2001), [33] performed dynamic testing and linear elastic finite element simulations of a similar PCB considering all the attached components. However the author did not consider the solder joints. In that study the natural frequencies and modal shapes of the PCB were measured and calculated with a 3D finite element model and the average stiffness and effective Young s modulus for different parts of the structure were measured. From the Pitarresi (2001), [33] analysis it is apparent that the fundamental mode of the structure induces flexure at the chipset and the processor locations. This is consistent with damage observed in the BGA solder joints during transportation. The corresponding finite element mesh is shown in Figure 1. In the first analysis set, we applied dynamic loading with amplitudes representative of those typically encountered during the service life, at 3 different frequencies and under isothermal conditions at room temperature. The dynamic loading was applied in the horizontal direction by imposing an acceleration history at the supported ends. A schematic of the applied dynamic load is shown in Figure 2. Second, we applied thermal loads only with the profile shown in Figure 3. In the final set of
8 316 Juan Gomez, Minghui Lin and Cemal Basaran analyses we applied the dynamic and thermal loads concurrently. The package was fully fixed at the ends, and the dynamic loading in form of input acceleration was prescribed at the support points and in the vertical direction. Modal analysis was performed first to determine the natural dynamic properties of the package. The first 5 modes are presented in Figure 4. Table 2 shows the first five natural frequencies of the structure. For the dynamical response an implicit direct integration scheme was used. The applied loads were harmonics with frequencies of 1Hz, 45Hz and 100Hz. Tab.1 Material properties for the elastic components Material E (GPa) σ y (MPa) ν ρ (tonne/mm^3) Pb37/Sn E09 BT E09 FR E09 UL 94V E09 Tab.2 Free vibration frequencies for the structure Mode Frequency(Hz) unloaded (a) (b)
9 Damage Mechanics Modeling of Concurrent Thermal. 317 Fig.1 (a) Complete Finite Element Model. (b) Mesh at the chipsetpcb region. Dynamic Loading 1.5 Support acceleration (g) Time (s) Fig.2 Schematic of the applied dynamic load. Thermal cycle Temperature Time (minutes) Fig.3 Schematic of the applied thermal profile.
10 318 Juan Gomez, Minghui Lin and Cemal Basaran Fig.4 Modal shapes of the first 5 modes
11 Damage Mechanics Modeling of Concurrent Thermal RESULTS AND DISCUSSION Figure 5 shows the relative displacement history at the center of the chipset for the studied frequencies. Figures 6a and 6b show the equivalent plastic strain induced by vibrations at 45Hz with two different time windows. The shown results are for the mostleft solder joint in Figure 1b. At the 1Hz and 100Hz frequencies there is no vibration induced plastic strain. Figure 7 shows the history of Von Misses equivalent stress for all the frequencies and for the thermal loading case at the same solder joint. Clearly the thermal solution alone overwhelms the Misses stresses even for the near resonance frequency of 45Hz. The equivalent plastic strain for the same loading case as in Figure 7 is shown in Figure 8. There is plastic strain at the 45Hz vibration but is almost negligible as compared to the thermal solution. In order to evaluate the validity of Miners rule we added the contributions from the independent thermal and vibration analysis and labeled this result Miners in the subsequent plots. For the 1.0Hz frequency under dynamic loads alone there is no plastic strain and the Miners solution and thermal solutions are exactly the same. Comparison with the concurrent solution at 1.0Hz is shown in Figure 9. The applied dynamic loading at this particular frequency caused no plastic strain, however it did increase the damage when applied concurrently with the thermal loading. Furthermore the concurrent loading generates larger plastic strains as compared to the thermal loading case. This result suggests that although the trend behind Miners rule is in the right direction (i.e., damage increases) the effect of the concurrent loading considerable increases damage and a linear superposition of both effects is inaccurate. Figure 10(a) and 10(b) present similar results for the 45Hz frequency for the equivalent plastic strain and Von Misses equivalent stress. In Figure 11 the case of 100Hz frequency is included in the results. Our results show that when the plastic strains due to independently applied vibrational and thermal loads are linearly added together to avoid the concurrent loading analysis the prediction underestimates the concurrent loading response. Therefore, from the computational results it can be concluded that using Miners rule leads to much smaller equivalent plastic strain and Misses stress values as compared to the concurrent application of the thermal and vibration loads.
12 320 Juan Gomez, Minghui Lin and Cemal Basaran Fig.5 1Hz, 45Hz, 100 Hz Dynamic loading only relative displacement. (a)
13 Damage Mechanics Modeling of Concurrent Thermal. 321 (b) Fig. 6 (a) 45Hz, Dynamic loading only equivalent plastic strain. (b) 45Hz, Dynamic loading only equivalent plastic strain. Fig.7 1Hz, 45Hz, 100Hz Dynamic and thermalmisses Stress
14 322 Juan Gomez, Minghui Lin and Cemal Basaran Fig.8 1Hz, 45Hz, 100Hz dynamic and thermalequivalent plastic strain. Fig.9 Equivalent plastic strain for the 1Hz Dynamic+thermal (Miners), concurrent and thermal load cases.
15 Damage Mechanics Modeling of Concurrent Thermal. 323 (a) (b) Fig.10 (a) Equivalent plastic strain for the 45Hz dynamic+thermal (Miners) and concurrent load cases. (b) Misses equivalent stress for the 45Hz dynamic+thermal (Miners) and concurrent load cases.
16 324 Juan Gomez, Minghui Lin and Cemal Basaran Fig.11 Equivalent plastic strain for the 1.0, 45.0 and 100Hz concurrent load case. 5. CONCLUSIONS AND RECOMMENDATIONS A damage mechanics coupled elastoviscoplastic constitutive model is proposed for analysis of microelectronic packaging under concurrent thermal and vibration loads. We have performed finite element analysis of electronic packaging under dynamic, thermal and concurrent (dynamic and thermal) load cases using a thermodynamics damage mechanics based rate dependent constitutive model for Pb/Sn solder alloys. The results from the simulations show that the superposition principle behind Miners rule that adds up the independent solutions from dynamic and thermal analysis to obtain the concurrent solution is correct for the boundary conditions and loading directions applied here. Yet, Miner s rule consistently underestimates the response of the system. The finite element simulations study conducted in here show that, using Miner s rule can lead to nonconservative results for certain boundary conditions and loading directions. ACKNOWLEDGMENTS This research project is supported by the United States Navy Office of Naval Research Advanced Electrical Power Systems Program, under the direction of director Terry Ericsen. REFERENCES
17 Damage Mechanics Modeling of Concurrent Thermal. 325 [1]. Kitano, B. P., Kawai, S. and Shimizu, L, Thermal Fatigue Strength Estimation of Solder Joints of Surface Mount IC Packages, Proc. 8 th Annual Int. Elec. Packaging Conf., IEPS, Dallas, Texas, pp.48, [2]. Lau, J. and Rice, J. R, Thermal Stress/ Strain Analyses of Ceramic Quad Flat Pack Packages and Interconnects, Elect. Components and Technology 40 th Conf., Vol.1, Los Vegas, Nevada, pp , [3]. Basaran, C., Chandaroy R. and Zhao, Y, Influence of Grain Size and Microstructure on Dynamic Response of Solder Joints, 98WA/EEP12, ASME Publications. [4]. Adams, P. J. Thermal Fatigue of Solder Joints in MicroElectronic Devices. M.S. thesis, Department of Mechanical Engineering, MIT, Cambridge, MA, [5]. Wilcox, J. R., Subrahmanyan, R., and Li, C. Thermal Stress Cycles and Inelastic Deformation in Solder Joints. Proc. 2 nd ASME Int. Electronic Mat. and Processing Congr., Philadelphis, PA, pp [6]. Knocht, S. and Fox. L. R. Constitutive Relation and CreepFatigue Life Model for Eutectic Tin Lead Solder. IEEE Trans Comp. Hybrids Manuf. Technol, 13 (1990) [7]. Darveaux, R. and Banerji, K. Constitutive Relations for TinBased Solder Joints. IEEE Trans. Comp. Hybrids Manuf. Technol, 15(1992) [8]. Hong, B. Z. and Burrell, L. G. Nonlinear Finite Element Simulation of Thermoviscoplastic Deformation of C4 Solder Joints in High Density Packaging Under Thermal Cycling. IEEE Trans. Components, Packaging, and Manufacturing TechnologyPart A, 18(1995) [9]. McDowell, D. L., Miller, M. P., and Brooks, D. C. A Unified CreepPlasticity Theory for Solder Alloys. Fatigue Testing of Electronic Materials, ASTM STP, 1153 (1994) [10]. Zhao, Y.. Thermomechanical Behavior of Ball Grid Array Solder Joints Under Thermal and Vibration Loading; Testing and Modeling. PhD Dissertation. University at Buffalo. The State University of New York, [11]. Basaran, C., and Tang, H., Implementation of a thermodynamic framework for damage mechanics of solder interconnect in microelectronic packaging. Proceedings of IMECE, 2002 ASME International Mechanical Engineering Congress & Exposition., New Orleans, Louisiana. [12]. Tang, H. A Thermodynamic Damage Mechanics Theory and Experimental Verification for Thermomechanical Fatigue Life Prediction of Microelectronics Solder Joints. PhD Dissertation. University at Buffalo. The State University of New York [13]. Kashyap, B., and Murty, G.. Experimental Constitutive Relations for the High Temperature Deformation of a PbSn Eutectic Alloy. Mater.Sci. and Engin, 50(1981) [14]. Gomez, J., and Basaran, C. Determination Of The Strain Gradient Plasticity Length Scale For Microelectronics Solder Alloys. Submitted to Inter. J. Plasticity. [15]. Gomez, J., and Basaran, C. Nanoindentation of Pb/Sn Solder Alloys;Experimental and Finite Element Simulation Results. Inter. J.Solids and Struc. in press [16]. Steinberg, D.S. Vibration Analysis for Electronic Equipment. 2 nd Edition., John Wiley & Sons, New York. (1988) [17]. Basaran, C., Zhao, Y., Tang, H., and Gomez, J. A Damage Mechanics Based Constitutive Model for Joints. ASME J. Electronic Packaging, 127 (2005) 17. [18]. Simo, J., and Hughes, T. Computational Inelasticity. Interdisciplinary applied mathematics. Springer [19]. Owen, D.R.J. and Hinton, E.. Finite Element in Plasticity, Pineridge Press Limited, Swansea, U.K [20]. Zhao, Y., Basaran, C., Cartwright, A., and Dishongh, T. Thermomechanical Behavior of Micron Scale Solder Joints: An Experimental Observation. J. Mech. Behavior of Mater, 10(1999) [21]. Barker, D., Vodzak, J., Dashgupta, A., and Pecht, M. Combined Vibrational and Thermal Solder Joint Fatigue. A Generalized Strain versus Life Approach. ASME J. Elec. Packaging, 2(1990) [22]. Miner, M.A. Cumulative Damage in Fatigue. ASME J. Applied Mech [23]. Lubarda, V and Benson, D.. On the numerical algorithm for isotropickinematic hardening with the ArmstrongFrederick evolution of the back stress. Comput. Methods Appl. Mech. Engrg, 191(2002)
18 326 Juan Gomez, Minghui Lin and Cemal Basaran [24]. Alfano, G., De Angelis, F., and Rosati, L. General Solution Procedures in Elasto/Viscoplasticity. Comput. Meth. Appl. Mech. Eng, 190(2001) [25]. Chaboche, J. Constitutive equations for cyclic plasticity and viscoplasticity. Inter. J. Plasticity, 3(1989) [26]. Armstrong, P. J., and Frederick, C. O. A Mathematical Representation of the Multiaxial Bauschinger Effect. CEGB Report RD/B/N [27]. Prager, W. A new method of analyzing stress and strains in workhardening plastic solids. Journal of Applied Mechanics, 23 (1956) [28]. Lemaitre, J. A course on damage mechanics.springerverlag. Germany [29]. Basaran, C., and Yan, C. A Thermodynamic Framework for Damage Mechanics of Solder Joints. Journal of Electronic Packaing, Trans. ASME, 120(1998) [30]. Basaran, C., and Nie, S. An Irreversible Thermodynamic Theory for Damage Mechanics of Solids. International Journal of Damage Mechanics, 13(2004) [31]. Gomez, J and Basaran, C. Numerical Simulation of Monotonic and Fatigue Shear Testing of Thin Layer Solder Joints Using a Damage mechanics Based Constitutive Model. Proceedings 2003 ASME Mechanics and Materials Conference, Scottsdale, Arizona. [32]. Pecht, M., Agarwal, R., Mc Cluskey, P., Dishong, T., Javadpour, S. and Mohajan, R. Electronic packaging materials and their properties. CRC press [33]. Pitarresi, M. Estimating Shock and Vibration Response in Personal Computers. Yearly Report. Department of Mechanical Engineering, State University of New York at Binghamton, December
Review of the Present Status of Rotor Aerodynamics
WIND ENERGY Wind Energ., 1, 46±69 (1998) Review Article Review of the Present Status of Rotor Aerodynamics H. Snel,* Netherlands Energy Research Foundation, Petten, The Netherlands Key words: aerodynamics;
More informationHigh Strain R. 33. High Strain Rate and Impact Experiments. Part D 33
1 High Strain R 33. High Strain Rate and Impact Experiments Part D 33 K. T. Ramesh Experimental techniques for highstrainrate measurements and for the study of impactrelated problems are described. An
More informationIrreversibility and Heat Generation in the Computing Process
R. Landauer Irreversibility and Heat Generation in the Computing Process Abstract: It is argued that computing machines inevitably involve devices which perform logical functions that do not have a singlevalued
More informationComparative Study on Frequency and Time Domain Analyses for Seismic Site Response
Comparative Study on Frequency and Time Domain Analyses for Seismic Site Response Ciro Visone, Filippo Santucci de Magistris University of Molise Structural and Geotechnical Dynamic Laboratory STReGa via
More informationVoice Coil Impedance as a Function of Frequency and Displacement
Voice Coil Impedance as a Function of Frequency and Displacement Mark Dodd 1, Wolfgang Klippel, and Jack OcleeBrown. 3 1 KEF Audio UK (Ltd),Maidstone,Kent,ME15 6QP United Kingdom. Mark.dodd@KEF.com Klippel
More informationWMR Control Via Dynamic Feedback Linearization: Design, Implementation, and Experimental Validation
IEEE TRANSACTIONS ON CONTROL SYSTEMS TECHNOLOGY, VOL. 10, NO. 6, NOVEMBER 2002 835 WMR Control Via Dynamic Feedback Linearization: Design, Implementation, and Experimental Validation Giuseppe Oriolo, Member,
More informationLABORATORY TESTS OF ACTIVE SUSPENSION SYSTEM
Journal of KONES Powertrain and Transport, Vol. 18, No. 1 2011 LABORATORY TESTS OF ACTIVE SUSPENSION SYSTEM Jaros aw Konieczny AGH University of Science and Technology, Department of Process Control Mickiewicz
More informationEPSRC Research Project EP/G00028X/1. Environmental Assessment of Domestic Laundering. Final Modelling Report
ESRU Report EPSRC Research Project EP/G00028X/1 Environmental Assessment of Domestic Laundering Final Modelling Report Kelly N J K, Markopoulos A and Strachan P A March 2012 Energy Systems Research Unit
More informationSingleElectron Devices and Their Applications
SingleElectron Devices and Their Applications KONSTANTIN K. LIKHAREV, MEMBER, IEEE Invited Paper The goal of this paper is to review in brief the basic physics of singleelectron devices, as well as their
More informationColloidal Suspensions in Temperature Gradients with Mesoscopic Simulations
Colloidal Suspensions in Temperature Gradients with Mesoscopic Simulations I n a u g u r a l  D i s s e r t a t i o n zur Erlangung des Doktorgrades der MathematischNaturwissenschaftlichen Fakultät der
More informationCall Admission Control in Mobile Cellular Networks: A Comprehensive Survey
Call Admission Control in Mobile Cellular Networks: A Comprehensive Survey Majid Ghaderi and Raouf Boutaba School of Computer Science University of Waterloo Waterloo, Ontario N2L 3G1, Canada Tel: +519
More informationAxial Flow Compressor Mean Line Design
Axial Flow Compressor Mean Line Design Niclas Falck February 2008 Master Thesis Division of Thermal Power Engineering Department of Energy Sciences Lund University, Sweden Niclas Falck 2008 ISSN 02821990
More informationMODEL SELECTION FOR SOCIAL NETWORKS USING GRAPHLETS
MODEL SELECTION FOR SOCIAL NETWORKS USING GRAPHLETS JEANNETTE JANSSEN, MATT HURSHMAN, AND NAUZER KALYANIWALLA Abstract. Several network models have been proposed to explain the link structure observed
More informationInvited Talk: Introduction to ElectromigrationAware Physical Design
Invited Talk: Introduction to ElectromigrationAware Physical Design Jens Lienig 1st Author Dresden University 2nd Author of Technology 3rd Author 1st author's affiliation Institute of Electromechanical
More informationOverview of Missile Flight Control Systems
Overview of Missile Flight Control Systems Paul B. Jackson he flight control system is a key element that allows the missile to meet its system performance requirements. The objective of the flight control
More information106 IEEE COMMUNICATIONS SURVEYS & TUTORIALS, VOL. 11, NO. 2, SECOND QUARTER 2009. survivability.
106 IEEE COMMUNICATIONS SURVEYS & TUTORIALS, VOL. 11, NO. 2, SECOND QUARTER 2009 A Comparative Analysis of Network Dependability, Faulttolerance, Reliability, Security, and Survivability M. AlKuwaiti,
More informationDynamic Behaviour of Reinforced Concrete Frames Designed with Direct DisplacementBased Design
European School for Advanced Studies in Reduction of Seismic Risk Research Report No. ROSE/ Dynamic Behaviour of Reinforced Concrete Frames ed with Direct DisplacementBased by J. Didier Pettinga Graduate
More informationTipping point failure and robustness in single development projects
Tipping point failure and robustness in single development projects Tim Taylor a and David N. Ford a * T. Taylor and D. N. Ford: Tipping Point Failure and Robustness 51 Tim Taylor is a PhD Candidate in
More informationUNIVERSITA DEGLI STUDI DI TRENTO Facoltà di Scienze Matematiche, Fisiche e Naturali
UNIVERSITA DEGLI STUDI DI TRENTO Facoltà di Scienze Matematiche, Fisiche e Naturali Corso di Laurea Magistrale in Informatica within European Master in Informatics Final Thesis OPTIMAL RELAY NODE PLACEMENT
More informationNeural Networks as Cybernetic Systems
 Neural Networks as Cybernetic Systems 2 nd and revised edition Holk Cruse Neural Networks as Cybernetic Systems 2 nd and revised edition Holk Cruse, Dr. Department of Biological Cybernetics and Theoretical
More informationTHE TWO major steps in applying any heuristic search algorithm
124 IEEE TRANSACTIONS ON EVOLUTIONARY COMPUTATION, VOL. 3, NO. 2, JULY 1999 Parameter Control in Evolutionary Algorithms Ágoston Endre Eiben, Robert Hinterding, and Zbigniew Michalewicz, Senior Member,
More informationDynamic Effect in the Capillary Pressure Saturation Relationship and its Impacts on Unsaturated Flow
Dynamic Effect in the Capillary Pressure Saturation Relationship and its Impacts on Unsaturated Flow S. Majid Hassanizadeh,* Michael A. Celia, and Helge K. Dahle ABSTRACT Capillary pressure plays a central
More informationHighDimensional Image Warping
Chapter 4 HighDimensional Image Warping John Ashburner & Karl J. Friston The Wellcome Dept. of Imaging Neuroscience, 12 Queen Square, London WC1N 3BG, UK. Contents 4.1 Introduction.................................
More informationChapter  E ROCK MECHANICS & GEOTECHNICAL APPLICATIONS
Chapter  E ROCK MECHANICS & GEOTECHNICAL APPLICATIONS 454 23 rd Effect of the Stress State on Waterjet Performance in Rock Slotting R. Ciccu, B. Grosso Department of Civil and Environmental Engineering
More informationUniversität Karlsruhe (TH) Institut für Baustatik
Universität Karlsruhe (TH) Institut für Baustatik A piezoelectric 3Dbeam finite element formulation accounting for geometrical and material nonlinearities A. Butz, S. Klinkel, W. Wagner Mitteilung 4(2007)
More informationFinal Draft of the original manuscript:
Final Draft of the original manuscript: Hilgert, J.; dos Santos, J.F.; Huber, N.: Shear layer modelling for bobbin tool friction stir welding In: Science and Technology of Welding and Joining (2012) Maney
More informationApplication of CFD in Membrane Technique
Application of CFD in Membrane Technique Der Fakultät für Ingenieurwissenschaften, Abteilung Maschinenbau der Universität DuisburgEssen zur Erlangung des akademischen Grades DOKTORINGENIEUR genehmigte
More informationAnalysis of EndtoEnd Response Times of MultiTier Internet Services
Analysis of EndtoEnd Response Times of MultiTier Internet Services ABSTRACT Modern Internet systems have evolved from simple monolithic systems to complex multitiered architectures For these systems,
More information1. Adaptation of cases for casebased forecasting with neural network support
1. Adaptation of cases for casebased forecasting with neural network support Corchado J. M. Artificial Intelligence Research Group Escuela Superior de Ingeniería Informática, University of Vigo, Campus
More informationTHE PROBLEM OF finding localized energy solutions
600 IEEE TRANSACTIONS ON SIGNAL PROCESSING, VOL. 45, NO. 3, MARCH 1997 Sparse Signal Reconstruction from Limited Data Using FOCUSS: A Reweighted Minimum Norm Algorithm Irina F. Gorodnitsky, Member, IEEE,
More information